#------------------------------------------------------------------------------
#$Date: 2016-03-23 22:28:48 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179482 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/79/4337904.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4337904
loop_
_publ_author_name
'Ogo, Shuhei'
'Shimizu, Noriko'
'Nishiki, Kensuke'
'Yasuda, Nobuhiro'
'Mizuta, Tsutomu'
'Sano, Tsuneji'
'Sadakane, Masahiro'
_publ_section_title
;
 Preparation and Redox Studies of α1- and α2-Isomers of
 Mono-Ru-Substituted Dawson-type Phosphotungstates with a DMSO Ligand:
 [α1/α2-P2W17O61Ru(II)(DMSO)](8-)
;
_journal_issue                   7
_journal_name_full               'Inorganic chemistry'
_journal_page_first              3526
_journal_paper_doi               10.1021/ic403041s
_journal_volume                  53
_journal_year                    2014
_chemical_formula_moiety
'(K +)8, (P2 W17 O61 Ru 8-), (C2 H6 O S), 16(H2 O)'
_chemical_formula_sum            'C2 H38 K8 O78 P2 Ru S W17'
_chemical_formula_weight         4943.64
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           11
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_atom_sites_solution_hydrogens   no
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 115.395(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   13.173(2)
_cell_length_b                   20.597(4)
_cell_length_c                   14.857(3)
_cell_measurement_temperature    123
_cell_volume                     3641.6(12)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      123
_diffrn_detector_area_resol_mean 8.333
_diffrn_measured_fraction_theta_full 0.978
_diffrn_measured_fraction_theta_max 0.978
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0561
_diffrn_reflns_av_sigmaI/netI    0.0756
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            21081
_diffrn_reflns_theta_full        27.85
_diffrn_reflns_theta_max         27.85
_diffrn_reflns_theta_min         1.52
_exptl_absorpt_coefficient_mu    27.580
_exptl_absorpt_correction_T_max  0.7700
_exptl_absorpt_correction_T_min  0.0959
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details
;
SADABS Sheldrick 1996
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.509
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             4348
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.01
_refine_diff_density_max         5.638
_refine_diff_density_min         -3.003
_refine_diff_density_rms         0.449
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.044
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     510
_refine_ls_number_reflns         8720
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.044
_refine_ls_R_factor_all          0.0848
_refine_ls_R_factor_gt           0.0552
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0728P)²+69.1709P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1459
_refine_ls_wR_factor_ref         0.1649
_reflns_number_gt                6086
_reflns_number_total             8720
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic403041s_si_003.cif
_cod_data_source_block           shimizu
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 4337904--4337905.cif.
;
_cod_original_sg_symbol_H-M      P21/m
_cod_database_code               4337904
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'
'-x, -y, -z'
'x, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W -0.10170(5) 0.83147(3) 0.35288(5) 0.02833(16) Uani 1 1 d . . .
W2 W 0.27198(6) 0.83779(3) 0.21366(5) 0.02988(17) Uani 1 1 d . A .
W3 W 0.11146(6) 0.83087(3) 0.62263(5) 0.03270(17) Uani 1 1 d . . .
W4 W 0.09388(6) 0.91953(3) 0.28188(6) 0.03611(19) Uani 1 1 d . . .
W5 W 0.48716(6) 0.83943(3) 0.48586(5) 0.03320(18) Uani 1 1 d . . .
W6 W 0.30775(6) 0.92019(3) 0.55188(6) 0.0399(2) Uani 1 1 d . . .
W9 W -0.14926(6) 0.83220(4) 0.08592(6) 0.0445(2) Uani 1 1 d . . .
W8 W 0.59523(9) 0.7500 0.72690(8) 0.0518(3) Uani 1 2 d S . .
W7 W 0.41615(7) 0.83187(5) 0.79363(6) 0.0533(3) Uani 1 1 d . . .
Ru1 Ru 0.03110(15) 0.7500 0.03209(15) 0.0351(4) Uani 1 2 d S . .
P1 P 0.3084(4) 0.7500 0.5619(4) 0.0191(10) Uani 1 2 d S . .
P2 P 0.0822(4) 0.7500 0.2768(4) 0.0150(9) Uani 1 2 d S . .
S1 S 0.0552(7) 0.7500 -0.0950(6) 0.088(4) Uani 1 2 d SD . .
C70A C 0.200(2) 0.764(2) -0.071(2) 0.048(10) Uiso 0.50 1 d PD A -1
H70A H 0.2083 0.7601 -0.1327 0.072 Uiso 0.50 1 calc PR A -1
H70B H 0.2479 0.7320 -0.0224 0.072 Uiso 0.50 1 calc PR A -1
H70C H 0.2222 0.8078 -0.0432 0.072 Uiso 0.50 1 calc PR A -1
C2A C 0.024(3) 0.6711(15) -0.151(3) 0.041(9) Uiso 0.50 1 d PD . -1
H2A1 H -0.0211 0.6469 -0.1240 0.062 Uiso 0.50 1 calc PR . -1
H2A2 H 0.0941 0.6477 -0.1358 0.062 Uiso 0.50 1 calc PR . -1
H2A3 H -0.0185 0.6756 -0.2231 0.062 Uiso 0.50 1 calc PR . -1
O2B O -0.020(5) 0.799(3) -0.182(4) 0.132(18) Uiso 0.50 1 d P . -1
O1 O -0.0073(10) 0.8222(5) 0.4955(8) 0.032(2) Uani 1 1 d . . .
O2 O 0.2170(10) 0.9258(5) 0.4119(10) 0.041(3) Uani 1 1 d . . .
O3 O 0.3815(9) 0.8537(5) 0.3570(8) 0.033(3) Uani 1 1 d . . .
O4 O 0.4410(12) 0.9175(6) 0.5286(10) 0.047(3) Uani 1 1 d . . .
O5 O 0.1806(10) 0.8892(6) 0.5683(10) 0.044(3) Uani 1 1 d . . .
O6 O 0.6063(10) 0.8679(7) 0.4767(10) 0.049(3) Uani 1 1 d . . .
O7 O 0.3285(9) 0.8113(5) 0.5143(9) 0.031(2) Uani 1 1 d . . .
O8 O 0.5630(9) 0.8141(7) 0.6279(9) 0.041(3) Uani 1 1 d . . .
O9 O 0.3943(11) 0.8892(7) 0.6871(10) 0.051(4) Uani 1 1 d . . .
O10 O 0.2566(10) 0.8262(6) 0.7363(9) 0.041(3) Uani 1 1 d . . .
O11 O 0.4432(13) 0.8832(10) 0.8908(11) 0.082(6) Uani 1 1 d . . .
O12 O 0.0503(11) 0.8835(6) 0.6736(10) 0.049(3) Uani 1 1 d . . .
O13 O -0.1983(10) 0.8834(6) 0.3622(10) 0.043(3) Uani 1 1 d . . .
O14 O -0.1614(10) 0.8277(6) 0.2154(9) 0.039(3) Uani 1 1 d . . .
O15 O 0.2005(11) 0.9168(5) 0.2269(10) 0.042(3) Uani 1 1 d . . .
O16 O 0.0095(9) 0.8886(5) 0.3512(9) 0.035(3) Uani 1 1 d . . .
O17 O 0.3585(11) 0.8681(7) 0.1623(11) 0.050(3) Uani 1 1 d . . .
O18 O -0.0877(12) 0.8195(7) -0.0004(10) 0.054(4) Uani 1 1 d . . .
O19 O 0.1527(10) 0.8156(6) 0.1020(9) 0.042(3) Uani 1 1 d . . .
O20 O 0.0613(13) 1.0005(6) 0.2678(12) 0.057(4) Uani 1 1 d . . .
O21 O -0.2553(12) 0.8873(8) 0.0244(11) 0.061(4) Uani 1 1 d . . .
O22 O 0.1535(8) 0.8115(5) 0.2927(7) 0.024(2) Uani 1 1 d . . .
O23 O 0.5626(11) 0.8151(9) 0.8058(10) 0.061(4) Uani 1 1 d . . .
O24 O -0.0249(10) 0.8901(6) 0.1628(9) 0.042(3) Uani 1 1 d . . .
O25 O 0.3082(13) 1.0005(7) 0.5796(13) 0.069(5) Uani 1 1 d . . .
O26 O 0.1939(12) 0.7500 0.5637(12) 0.028(3) Uani 1 2 d S . .
O27 O 0.4920(13) 0.7500 0.4617(13) 0.037(4) Uani 1 2 d S . .
O28 O 0.3978(14) 0.7500 0.6754(12) 0.038(4) Uani 1 2 d S . .
O29 O 0.0742(13) 0.7500 0.6638(12) 0.035(4) Uani 1 2 d S . .
O30 O -0.1663(14) 0.7500 0.3611(12) 0.035(4) Uani 1 2 d S . .
O31 O 0.3227(13) 0.7500 0.2456(12) 0.031(4) Uani 1 2 d S . .
O32 O -0.0106(11) 0.7500 0.1644(9) 0.026(3) Uani 1 2 d S . .
O33 O 0.4204(16) 0.7500 0.8566(15) 0.059(6) Uani 1 2 d S . .
O34 O -0.2241(14) 0.7500 0.0623(16) 0.052(5) Uani 1 2 d S . .
O35 O 0.7398(17) 0.7500 0.7856(16) 0.078(8) Uani 1 2 d S . .
O36 O 0.0186(12) 0.7500 0.3419(11) 0.027(3) Uani 1 2 d S . .
K1 K 0.1739(5) 1.0843(3) 0.4394(5) 0.0832(19) Uani 1 1 d . . .
K2 K 0.5738(4) 0.9028(3) 0.2873(4) 0.0706(15) Uani 1 1 d . . .
K3 K 0.1584(15) 0.9954(6) 0.7091(17) 0.082(6) Uani 0.35 1 d P . .
K4 K 0.224(2) 1.1125(13) 0.1825(13) 0.129(10) Uani 0.34 1 d P . .
K6 K 0.356(2) 0.961(2) 0.0163(18) 0.183(17) Uani 0.35 1 d P . .
O37 O 0.0000 1.0000 0.5000 0.074(7) Uiso 1 2 d S . .
O38 O 0.226(3) 1.2272(17) 0.476(3) 0.081(16) Uiso 0.47(4) 1 d P . .
O39 O 0.417(2) 0.9930(13) 0.3275(19) 0.057(10) Uiso 0.55(5) 1 d P . .
O40 O 0.344(3) 1.0260(18) 0.350(3) 0.046(14) Uiso 0.35(4) 1 d P . .
O43 O 0.599(4) 0.942(2) 0.119(3) 0.14(2) Uiso 0.63(6) 1 d P . .
O44 O 0.573(3) 0.7500 0.294(2) 0.115(11) Uiso 1 2 d S . .
K5 K 0.370(3) 1.0396(17) 0.135(2) 0.162(16) Uani 0.31 1 d P . .
O46 O 0.578(5) 0.850(3) 0.114(5) 0.26(4) Uiso 0.79(10) 1 d P . .
O41 O 0.1183(15) 0.9481(9) -0.1435(13) 0.024(6) Uiso 0.52(4) 1 d P . .
O45 O 0.248(5) 1.000(3) 0.766(4) 0.01(2) Uiso 0.14(4) 1 d P . .
O47 O 0.422(3) 0.7500 0.076(3) 0.010(14) Uiso 0.27(5) 2 d SP . .
O48 O 0.179(5) 1.167(3) 0.337(4) 0.18(3) Uiso 0.62(8) 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ru Ru -1.2594 0.8363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O13 W1 O14 97.9(6) . .
O13 W1 O16 102.7(5) . .
O14 W1 O16 88.6(5) . .
O13 W1 O30 100.1(6) . .
O14 W1 O30 92.5(6) . .
O16 W1 O30 156.8(5) . .
O13 W1 O1 97.1(6) . .
O14 W1 O1 164.9(5) . .
O16 W1 O1 86.5(5) . .
O30 W1 O1 86.5(6) . .
O13 W1 O36 173.3(5) . .
O14 W1 O36 82.7(5) . .
O16 W1 O36 84.0(4) . .
O30 W1 O36 73.2(5) . .
O1 W1 O36 82.6(5) . .
O13 W1 K3 48.5(5) . 3_576
O14 W1 K3 79.6(5) . 3_576
O16 W1 K3 57.8(4) . 3_576
O30 W1 K3 145.1(5) . 3_576
O1 W1 K3 109.4(5) . 3_576
O36 W1 K3 137.9(4) . 3_576
O13 W1 K1 40.1(5) . 3_576
O14 W1 K1 138.0(4) . 3_576
O16 W1 K1 100.5(4) . 3_576
O30 W1 K1 94.1(4) . 3_576
O1 W1 K1 57.1(3) . 3_576
O36 W1 K1 138.7(4) . 3_576
K3 W1 K1 71.5(3) 3_576 3_576
O17 W2 O19 99.5(6) . .
O17 W2 O31 102.9(6) . .
O19 W2 O31 93.6(6) . .
O17 W2 O15 100.5(6) . .
O19 W2 O15 92.1(6) . .
O31 W2 O15 154.6(5) . .
O17 W2 O3 95.6(6) . .
O19 W2 O3 164.8(5) . .
O31 W2 O3 82.9(6) . .
O15 W2 O3 85.1(5) . .
O17 W2 O22 171.8(5) . .
O19 W2 O22 84.2(4) . .
O31 W2 O22 84.1(5) . .
O15 W2 O22 72.0(4) . .
O3 W2 O22 80.8(4) . .
O17 W2 K2 38.2(5) . .
O19 W2 K2 137.4(4) . .
O31 W2 K2 92.8(4) . .
O15 W2 K2 99.5(4) . .
O3 W2 K2 57.7(3) . .
O22 W2 K2 138.4(3) . .
O12 W3 O1 99.1(6) . .
O12 W3 O5 101.1(6) . .
O1 W3 O5 88.6(5) . .
O12 W3 O29 100.2(6) . .
O1 W3 O29 91.3(6) . .
O5 W3 O29 158.5(5) . .
O12 W3 O10 97.0(6) . .
O1 W3 O10 163.7(5) . .
O5 W3 O10 85.9(5) . .
O29 W3 O10 88.3(6) . .
O12 W3 O26 173.9(6) . .
O1 W3 O26 82.9(5) . .
O5 W3 O26 84.7(4) . .
O29 W3 O26 74.0(5) . .
O10 W3 O26 81.3(5) . .
O12 W3 K3 44.2(5) . .
O1 W3 K3 113.1(5) . .
O5 W3 K3 60.7(5) . .
O29 W3 K3 137.7(5) . .
O10 W3 K3 77.3(5) . .
O26 W3 K3 140.1(4) . .
O12 W3 K1 39.4(5) . 3_576
O1 W3 K1 59.9(3) . 3_576
O5 W3 K1 102.0(4) . 3_576
O29 W3 K1 96.5(4) . 3_576
O10 W3 K1 136.3(4) . 3_576
O26 W3 K1 141.7(4) . 3_576
K3 W3 K1 70.1(3) . 3_576
O20 W4 O24 97.7(7) . .
O20 W4 O15 99.7(6) . .
O24 W4 O15 93.2(5) . .
O20 W4 O16 102.5(6) . .
O24 W4 O16 87.6(5) . .
O15 W4 O16 157.5(5) . .
O20 W4 O2 96.7(6) . .
O24 W4 O2 165.0(5) . .
O15 W4 O2 88.5(6) . .
O16 W4 O2 85.2(5) . .
O20 W4 O22 173.1(5) . .
O24 W4 O22 83.0(4) . .
O15 W4 O22 73.4(4) . .
O16 W4 O22 84.4(4) . .
O2 W4 O22 83.2(4) . .
O20 W4 K3 51.7(5) . 3_576
O24 W4 K3 78.2(5) . 3_576
O15 W4 K3 147.5(4) . 3_576
O16 W4 K3 54.5(4) . 3_576
O2 W4 K3 107.8(5) . 3_576
O22 W4 K3 134.9(3) . 3_576
O20 W4 K1 40.0(6) . .
O24 W4 K1 136.4(4) . .
O15 W4 K1 102.6(4) . .
O16 W4 K1 92.0(4) . .
O2 W4 K1 57.2(3) . .
O22 W4 K1 140.3(3) . .
K3 W4 K1 66.7(3) 3_576 .
O6 W5 O3 99.8(6) . .
O6 W5 O27 102.1(6) . .
O3 W5 O27 91.7(6) . .
O6 W5 O4 99.7(6) . .
O3 W5 O4 90.3(6) . .
O27 W5 O4 157.4(6) . .
O6 W5 O8 96.4(5) . .
O3 W5 O8 163.7(5) . .
O27 W5 O8 84.4(6) . .
O4 W5 O8 87.4(6) . .
O6 W5 O7 172.5(5) . .
O3 W5 O7 83.9(4) . .
O27 W5 O7 84.2(5) . .
O4 W5 O7 73.6(4) . .
O8 W5 O7 80.0(4) . .
O6 W5 K2 40.9(4) . .
O3 W5 K2 59.1(3) . .
O27 W5 K2 98.1(5) . .
O4 W5 K2 102.2(4) . .
O8 W5 K2 137.0(3) . .
O7 W5 K2 142.9(3) . .
O25 W6 O5 101.9(6) . .
O25 W6 O2 98.1(7) . .
O5 W6 O2 89.1(6) . .
O25 W6 O4 99.3(6) . .
O5 W6 O4 158.6(5) . .
O2 W6 O4 90.0(6) . .
O25 W6 O9 97.4(7) . .
O5 W6 O9 85.2(6) . .
O2 W6 O9 164.3(5) . .
O4 W6 O9 90.0(6) . .
O25 W6 O7 173.2(5) . .
O5 W6 O7 84.8(4) . .
O2 W6 O7 83.2(4) . .
O4 W6 O7 73.9(4) . .
O9 W6 O7 81.7(5) . .
O25 W6 K1 37.4(6) . .
O5 W6 K1 94.9(4) . .
O2 W6 K1 61.1(3) . .
O4 W6 K1 103.3(4) . .
O9 W6 K1 133.9(4) . .
O7 W6 K1 144.3(3) . .
O25 W6 K3 55.1(6) . .
O5 W6 K3 50.8(4) . .
O2 W6 K3 112.5(5) . .
O4 W6 K3 146.9(4) . .
O9 W6 K3 74.8(5) . .
O7 W6 K3 130.6(3) . .
K1 W6 K3 70.2(3) . .
O21 W9 O18 103.1(6) . .
O21 W9 O34 104.4(7) . .
O18 W9 O34 95.4(8) . .
O21 W9 O24 101.2(6) . .
O18 W9 O24 89.1(6) . .
O34 W9 O24 152.3(6) . .
O21 W9 O14 99.2(6) . .
O18 W9 O14 157.2(5) . .
O34 W9 O14 83.6(7) . .
O24 W9 O14 81.9(5) . .
O21 W9 O32 176.1(6) . .
O18 W9 O32 76.2(5) . .
O34 W9 O32 71.9(5) . .
O24 W9 O32 82.7(4) . .
O14 W9 O32 81.8(5) . .
O21 W9 K4 57.8(7) . 3_575
O18 W9 K4 45.6(6) . 3_575
O34 W9 K4 100.9(8) . 3_575
O24 W9 K4 101.7(5) . 3_575
O14 W9 K4 157.0(6) . 3_575
O32 W9 K4 121.1(6) . 3_575
O35 W8 O8 103.0(6) . .
O35 W8 O8 103.0(6) . 4_575
O8 W8 O8 88.9(7) . 4_575
O35 W8 O23 100.2(7) . 4_575
O8 W8 O23 156.7(5) . 4_575
O8 W8 O23 87.3(6) 4_575 4_575
O35 W8 O23 100.2(7) . .
O8 W8 O23 87.3(6) . .
O8 W8 O23 156.7(5) 4_575 .
O23 W8 O23 87.1(10) 4_575 .
O35 W8 O28 169.7(8) . .
O8 W8 O28 84.3(4) . .
O8 W8 O28 84.3(4) 4_575 .
O23 W8 O28 72.5(5) 4_575 .
O23 W8 O28 72.5(5) . .
O35 W8 K4 52.7(5) . 3_676
O8 W8 K4 68.2(4) . 3_676
O8 W8 K4 137.7(6) 4_575 3_676
O23 W8 K4 127.1(5) 4_575 3_676
O23 W8 K4 60.7(7) . 3_676
O28 W8 K4 125.6(5) . 3_676
O35 W8 K4 52.7(5) . 2_646
O8 W8 K4 137.7(6) . 2_646
O8 W8 K4 68.2(4) 4_575 2_646
O23 W8 K4 60.7(7) 4_575 2_646
O23 W8 K4 127.1(5) . 2_646
O28 W8 K4 125.6(5) . 2_646
K4 W8 K4 104.9(9) 3_676 2_646
O11 W7 O23 101.5(7) . .
O11 W7 O9 102.9(8) . .
O23 W7 O9 88.7(7) . .
O11 W7 O10 102.0(7) . .
O23 W7 O10 156.5(6) . .
O9 W7 O10 85.5(6) . .
O11 W7 O33 100.5(9) . .
O23 W7 O33 88.7(8) . .
O9 W7 O33 156.6(6) . .
O10 W7 O33 87.7(7) . .
O11 W7 O28 171.6(8) . .
O23 W7 O28 73.5(6) . .
O9 W7 O28 83.9(5) . .
O10 W7 O28 83.3(5) . .
O33 W7 O28 73.0(6) . .
O11 W7 K5 56.7(9) . 3_676
O23 W7 K5 58.6(9) . 3_676
O9 W7 K5 67.3(5) . 3_676
O10 W7 K5 137.4(7) . 3_676
O33 W7 K5 129.4(7) . 3_676
O28 W7 K5 123.2(8) . 3_676
O19 Ru1 O19 84.4(7) 4_575 .
O19 Ru1 O18 90.6(6) 4_575 4_575
O19 Ru1 O18 164.4(5) . 4_575
O19 Ru1 O18 164.4(5) 4_575 .
O19 Ru1 O18 90.6(6) . .
O18 Ru1 O18 90.2(9) 4_575 .
O19 Ru1 S1 94.1(4) 4_575 .
O19 Ru1 S1 94.1(4) . .
O18 Ru1 S1 101.0(4) 4_575 .
O18 Ru1 S1 101.0(4) . .
O19 Ru1 O32 89.3(4) 4_575 .
O19 Ru1 O32 89.3(4) . .
O18 Ru1 O32 75.8(4) 4_575 .
O18 Ru1 O32 75.8(4) . .
S1 Ru1 O32 175.4(4) . .
O26 P1 O7 112.3(5) . .
O26 P1 O7 112.3(5) . 4_575
O7 P1 O7 111.8(9) . 4_575
O26 P1 O28 105.7(9) . .
O7 P1 O28 107.2(6) . .
O7 P1 O28 107.2(6) 4_575 .
O36 P2 O22 111.6(5) . .
O36 P2 O22 111.6(5) . 4_575
O22 P2 O22 111.4(8) . 4_575
O36 P2 O32 106.3(8) . .
O22 P2 O32 107.8(5) . .
O22 P2 O32 107.8(5) 4_575 .
O2B S1 O2B 78(4) . 4_575
O2B S1 C2A 28(2) . 4_575
O2B S1 C2A 105(3) 4_575 4_575
O2B S1 C2A 105(3) . .
O2B S1 C2A 28(2) 4_575 .
C2A S1 C2A 130(3) 4_575 .
O2B S1 C70A 107(2) . .
O2B S1 C70A 120(2) 4_575 .
C2A S1 C70A 87.8(18) 4_575 .
C2A S1 C70A 104.6(19) . .
O2B S1 C70A 120(2) . 4_575
O2B S1 C70A 107(2) 4_575 4_575
C2A S1 C70A 104.6(19) 4_575 4_575
C2A S1 C70A 87.8(18) . 4_575
C70A S1 C70A 18(3) . 4_575
O2B S1 Ru1 117(2) . .
O2B S1 Ru1 117(2) 4_575 .
C2A S1 Ru1 109.4(13) 4_575 .
C2A S1 Ru1 109.4(13) . .
C70A S1 Ru1 112.5(11) . .
C70A S1 Ru1 112.5(11) 4_575 .
S1 C70A H70A 109.5 . .
S1 C70A H70B 109.5 . .
S1 C70A H70C 109.5 . .
S1 C2A K4 114.4(18) . 2_545
S1 C2A H2A1 109.5 . .
K4 C2A H2A1 31.1 2_545 .
S1 C2A H2A2 109.5 . .
K4 C2A H2A2 128.9 2_545 .
S1 C2A H2A3 109.5 . .
K4 C2A H2A3 79.3 2_545 .
S1 O2B K4 125(3) . 3_575
W3 O1 W1 162.3(6) . .
W3 O1 K1 91.2(4) . 3_576
W1 O1 K1 93.8(4) . 3_576
W6 O2 W4 163.1(7) . .
W6 O2 K1 89.2(4) . .
W4 O2 K1 94.2(4) . .
W5 O3 W2 161.3(7) . .
W5 O3 K2 92.0(4) . .
W2 O3 K2 90.9(4) . .
W5 O4 W6 121.6(6) . .
W3 O5 W6 151.9(8) . .
W3 O5 K3 87.6(5) . .
W6 O5 K3 101.0(5) . .
W5 O6 K2 114.8(6) . .
W5 O6 K1 152.1(7) . 3_676
K2 O6 K1 92.3(4) . 3_676
P1 O7 W6 128.1(6) . .
P1 O7 W5 128.7(6) . .
W6 O7 W5 90.6(3) . .
W8 O8 W5 149.2(7) . .
W8 O8 K4 80.4(5) . 3_676
W5 O8 K4 129.3(7) . 3_676
W7 O9 W6 151.6(7) . .
W7 O9 K5 82.0(6) . 3_676
W6 O9 K5 126.3(7) . 3_676
W7 O10 W3 151.1(7) . .
W7 O11 K6 148.7(10) . 1_556
W7 O11 K5 95.9(10) . 3_676
K6 O11 K5 109.7(12) 1_556 3_676
W3 O12 K3 109.0(7) . .
W3 O12 K1 117.7(6) . 3_576
K3 O12 K1 104.7(6) . 3_576
W1 O13 K2 141.2(7) . 1_455
W1 O13 K3 104.8(6) . 3_576
K2 O13 K3 93.7(5) 1_455 3_576
W1 O13 K1 117.6(6) . 3_576
K2 O13 K1 90.2(4) 1_455 3_576
K3 O13 K1 102.6(6) 3_576 3_576
W1 O14 W9 152.8(7) . .
W4 O15 W2 123.3(5) . .
W1 O16 W4 147.7(7) . .
W1 O16 K3 91.3(5) . 3_576
W4 O16 K3 95.5(5) . 3_576
W2 O17 K2 118.7(7) . .
W2 O17 K6 140.4(8) . .
K2 O17 K6 90.6(7) . .
W9 O18 Ru1 118.1(6) . .
W9 O18 K4 107.9(8) . 3_575
Ru1 O18 K4 132.4(9) . 3_575
W2 O19 Ru1 147.1(7) . .
W4 O20 K1 117.7(8) . .
W4 O20 K3 102.3(6) . 3_576
K1 O20 K3 92.2(5) . 3_576
W9 O21 K5 149.8(13) . 3_575
W9 O21 K4 95.7(7) . 3_575
K5 O21 K4 54.2(11) 3_575 3_575
W9 O21 K6 151.4(10) . 3_575
K5 O21 K6 44.1(10) 3_575 3_575
K4 O21 K6 91.7(7) 3_575 3_575
P2 O22 W4 127.5(6) . .
P2 O22 W2 126.7(5) . .
W4 O22 W2 91.3(4) . .
W7 O23 W8 123.3(7) . .
W7 O23 K4 140.9(10) . 3_676
W8 O23 K4 86.3(7) . 3_676
W7 O23 K5 90.4(10) . 3_676
W8 O23 K5 135.7(10) . 3_676
K4 O23 K5 52.3(10) 3_676 3_676
W4 O24 W9 153.4(6) . .
W6 O25 K1 120.0(8) . .
W6 O25 K2 144.5(9) . 3_676
K1 O25 K2 94.2(5) . 3_676
W6 O25 K3 99.8(6) . .
K1 O25 K3 96.5(6) . .
K2 O25 K3 84.2(5) 3_676 .
P1 O26 W3 128.8(5) . .
P1 O26 W3 128.8(5) . 4_575
W3 O26 W3 90.2(5) . 4_575
W5 O27 W5 156.1(10) 4_575 .
P1 O28 W7 125.4(5) . .
P1 O28 W7 125.4(5) . 4_575
W7 O28 W7 90.7(5) . 4_575
P1 O28 W8 123.5(8) . .
W7 O28 W8 90.7(5) . .
W7 O28 W8 90.7(5) 4_575 .
W3 O29 W3 121.5(8) 4_575 .
W1 O30 W1 123.1(8) 4_575 .
W2 O31 W2 141.5(9) 4_575 .
P2 O32 Ru1 123.4(8) . .
P2 O32 W9 126.4(4) . 4_575
Ru1 O32 W9 89.7(4) . 4_575
P2 O32 W9 126.4(4) . .
Ru1 O32 W9 89.7(4) . .
W9 O32 W9 90.0(4) 4_575 .
W7 O33 W7 123.2(10) . 4_575
W9 O34 W9 124.4(9) . 4_575
W8 O35 K4 98.8(7) . 3_676
W8 O35 K4 98.8(7) . 2_646
K4 O35 K4 159.6(12) 3_676 2_646
P2 O36 W1 127.6(5) . .
P2 O36 W1 127.6(5) . 4_575
W1 O36 W1 90.6(5) . 4_575
O48 K1 O25 141.9(15) . .
O48 K1 O12 75.5(15) . 3_576
O25 K1 O12 142.5(5) . 3_576
O48 K1 O6 73.5(15) . 3_676
O25 K1 O6 70.8(4) . 3_676
O12 K1 O6 144.5(5) 3_576 3_676
O48 K1 O13 118.5(14) . 3_576
O25 K1 O13 67.2(4) . 3_576
O12 K1 O13 100.6(4) 3_576 3_576
O6 K1 O13 79.9(4) 3_676 3_576
O48 K1 O20 90.6(15) . .
O25 K1 O20 102.5(5) . .
O12 K1 O20 66.5(4) 3_576 .
O6 K1 O20 130.0(4) 3_676 .
O13 K1 O20 145.1(4) 3_576 .
O48 K1 O38 47.7(15) . .
O25 K1 O38 117.5(8) . .
O12 K1 O38 88.7(7) 3_576 .
O6 K1 O38 57.5(7) 3_676 .
O13 K1 O38 71.1(7) 3_576 .
O20 K1 O38 136.8(7) . .
O48 K1 O40 77.7(16) . .
O25 K1 O40 75.1(7) . .
O12 K1 O40 125.2(7) 3_576 .
O6 K1 O40 63.4(7) 3_676 .
O13 K1 O40 134.1(7) 3_576 .
O20 K1 O40 66.9(7) . .
O38 K1 O40 106.7(10) . .
O48 K1 O37 142.3(15) . .
O25 K1 O37 75.8(3) . .
O12 K1 O37 66.9(3) 3_576 .
O6 K1 O37 140.6(4) 3_676 .
O13 K1 O37 68.3(3) 3_576 .
O20 K1 O37 76.9(3) . .
O38 K1 O37 126.7(7) . .
O40 K1 O37 126.3(7) . .
O48 K1 O1 88.4(15) . 3_576
O25 K1 O1 115.9(4) . 3_576
O12 K1 O1 51.7(3) 3_576 3_576
O6 K1 O1 110.5(4) 3_676 3_576
O13 K1 O1 51.5(3) 3_576 3_576
O20 K1 O1 116.2(4) . 3_576
O38 K1 O1 61.1(7) . 3_576
O40 K1 O1 166.0(7) . 3_576
O37 K1 O1 66.8(2) . 3_576
O48 K1 O2 125.7(15) . .
O25 K1 O2 52.1(4) . .
O12 K1 O2 110.4(4) 3_576 .
O6 K1 O2 101.5(4) 3_676 .
O13 K1 O2 113.2(4) 3_576 .
O20 K1 O2 50.7(4) . .
O38 K1 O2 158.4(7) . .
O40 K1 O2 54.3(7) . .
O37 K1 O2 72.2(3) . .
O1 K1 O2 139.0(4) 3_576 .
O48 K1 W6 143.1(15) . .
O25 K1 W6 22.5(3) . .
O12 K1 W6 130.0(3) 3_576 .
O6 K1 W6 85.5(3) 3_676 .
O13 K1 W6 86.0(3) 3_576 .
O20 K1 W6 80.0(3) . .
O38 K1 W6 138.7(7) . .
O40 K1 W6 65.7(7) . .
O37 K1 W6 70.17(13) . .
O1 K1 W6 127.8(3) 3_576 .
O2 K1 W6 29.7(2) . .
O17 K2 O13 150.7(5) . 1_655
O17 K2 O6 106.7(4) . .
O13 K2 O6 83.3(4) 1_655 .
O17 K2 O25 140.7(5) . 3_676
O13 K2 O25 68.5(4) 1_655 3_676
O6 K2 O25 70.4(5) . 3_676
O17 K2 O43 87.5(10) . .
O13 K2 O43 82.8(10) 1_655 .
O6 K2 O43 165.6(10) . .
O25 K2 O43 100.6(10) 3_676 .
O17 K2 O46 72.7(13) . .
O13 K2 O46 82.3(13) 1_655 .
O6 K2 O46 141.0(14) . .
O25 K2 O46 134.8(14) 3_676 .
O43 K2 O46 40.1(15) . .
O17 K2 O39 72.3(6) . .
O13 K2 O39 137.0(6) 1_655 .
O6 K2 O39 77.2(6) . .
O25 K2 O39 68.9(6) 3_676 .
O43 K2 O39 110.8(11) . .
O46 K2 O39 134.6(14) . .
O17 K2 O44 75.2(7) . .
O13 K2 O44 81.9(7) 1_655 .
O6 K2 O44 73.0(7) . .
O25 K2 O44 134.9(7) 3_676 .
O43 K2 O44 108.9(12) . .
O46 K2 O44 69.1(15) . .
O39 K2 O44 126.5(8) . .
O17 K2 O3 54.4(3) . .
O13 K2 O3 133.2(4) 1_655 .
O6 K2 O3 53.1(3) . .
O25 K2 O3 105.6(4) 3_676 .
O43 K2 O3 141.3(10) . .
O46 K2 O3 119.4(14) . .
O39 K2 O3 56.0(6) . .
O44 K2 O3 70.6(7) . .
O17 K2 O45 127.7(10) . 3_676
O13 K2 O45 55.9(10) 1_655 3_676
O6 K2 O45 124.5(10) . 3_676
O25 K2 O45 60.9(10) 3_676 3_676
O43 K2 O45 42.6(13) . 3_676
O46 K2 O45 74.3(17) . 3_676
O39 K2 O45 106.5(11) . 3_676
O44 K2 O45 127.0(12) . 3_676
O3 K2 O45 162.2(10) . 3_676
O17 K2 W5 82.5(3) . .
O13 K2 W5 105.9(3) 1_655 .
O6 K2 W5 24.3(2) . .
O25 K2 W5 87.5(4) 3_676 .
O43 K2 W5 169.9(9) . .
O46 K2 W5 134.7(14) . .
O39 K2 W5 66.5(5) . .
O44 K2 W5 68.2(6) . .
O3 K2 W5 28.8(2) . .
O45 K2 W5 147.0(9) 3_676 .
O17 K2 K5 62.4(5) . .
O13 K2 K5 134.8(6) 1_655 .
O6 K2 K5 123.4(7) . .
O25 K2 K5 86.0(6) 3_676 .
O43 K2 K5 65.5(11) . .
O46 K2 K5 91.7(14) . .
O39 K2 K5 46.2(8) . .
O44 K2 K5 137.2(8) . .
O3 K2 K5 88.4(6) . .
O45 K2 K5 79.3(11) 3_676 .
W5 K2 K5 109.7(6) . .
O45 K3 O12 122(3) . .
O45 K3 O41 86(3) . 1_556
O12 K3 O41 64.0(6) . 1_556
O45 K3 O13 84(3) . 3_576
O12 K3 O13 149.4(10) . 3_576
O41 K3 O13 139.9(8) 1_556 3_576
O45 K3 O37 147(3) . .
O12 K3 O37 74.7(6) . .
O41 K3 O37 126.1(7) 1_556 .
O13 K3 O37 74.7(6) 3_576 .
O45 K3 O20 131(3) . 3_576
O12 K3 O20 65.8(5) . 3_576
O41 K3 O20 51.9(6) 1_556 3_576
O13 K3 O20 110.6(6) 3_576 3_576
O37 K3 O20 80.7(6) . 3_576
O45 K3 O16 122(3) . 3_576
O12 K3 O16 110.9(7) . 3_576
O41 K3 O16 98.7(6) 1_556 3_576
O13 K3 O16 56.1(4) 3_576 3_576
O37 K3 O16 64.7(5) . 3_576
O20 K3 O16 54.7(4) 3_576 3_576
O45 K3 O5 101(3) . .
O12 K3 O5 56.8(4) . .
O41 K3 O5 113.8(7) 1_556 .
O13 K3 O5 106.2(7) 3_576 .
O37 K3 O5 62.5(5) . .
O20 K3 O5 117.3(6) 3_576 .
O16 K3 O5 127.1(8) 3_576 .
O45 K3 O25 75(3) . .
O12 K3 O25 108.5(6) . .
O41 K3 O25 151.1(8) 1_556 .
O13 K3 O25 60.2(5) 3_576 .
O37 K3 O25 73.2(6) . .
O20 K3 O25 153.8(9) 3_576 .
O16 K3 O25 109.7(7) 3_576 .
O5 K3 O25 51.7(4) . .
O45 K3 O43 18(3) . 3_676
O12 K3 O43 137.5(11) . 3_676
O41 K3 O43 88.5(11) 1_556 3_676
O13 K3 O43 71.5(9) 3_576 3_676
O37 K3 O43 144.1(9) . 3_676
O20 K3 O43 122.6(10) 3_576 3_676
O16 K3 O43 104.5(9) 3_576 3_676
O5 K3 O43 116.4(9) . 3_676
O25 K3 O43 79.7(9) . 3_676
O45 K3 W3 109(3) . .
O12 K3 W3 26.8(3) . .
O41 K3 W3 83.3(5) 1_556 .
O13 K3 W3 136.6(7) 3_576 .
O37 K3 W3 73.3(4) . .
O20 K3 W3 92.3(4) 3_576 .
O16 K3 W3 129.1(7) 3_576 .
O5 K3 W3 31.7(3) . .
O25 K3 W3 82.8(4) . .
O43 K3 W3 126.4(9) 3_676 .
O45 K3 W1 98(3) . 3_576
O12 K3 W1 139.6(7) . 3_576
O41 K3 W1 118.2(6) 1_556 3_576
O13 K3 W1 26.8(3) 3_576 3_576
O37 K3 W1 74.1(4) . 3_576
O20 K3 W1 84.3(4) 3_576 3_576
O16 K3 W1 30.9(2) 3_576 3_576
O5 K3 W1 125.3(7) . 3_576
O25 K3 W1 86.1(5) . 3_576
O43 K3 W1 81.1(8) 3_676 3_576
W3 K3 W1 147.3(7) . 3_576
K5 K4 O48 146.3(15) . .
K5 K4 O35 119.5(13) . 3_676
O48 K4 O35 63.5(13) . 3_676
K5 K4 O18 104.2(9) . 3_575
O48 K4 O18 107.7(15) . 3_575
O35 K4 O18 70.7(8) 3_676 3_575
K5 K4 O40 72.8(11) . .
O48 K4 O40 77.0(14) . .
O35 K4 O40 118.0(11) 3_676 .
O18 K4 O40 171.2(13) 3_575 .
K5 K4 O23 64.2(9) . 3_676
O48 K4 O23 105.1(14) . 3_676
O35 K4 O23 55.8(7) 3_676 3_676
O18 K4 O23 90.2(8) 3_575 3_676
O40 K4 O23 95.7(11) . 3_676
K5 K4 O2B 166.6(12) . 3_575
O48 K4 O2B 47.1(16) . 3_575
O35 K4 O2B 61.9(13) 3_676 3_575
O18 K4 O2B 62.9(11) 3_575 3_575
O40 K4 O2B 119.3(15) . 3_575
O23 K4 O2B 117.3(14) 3_676 3_575
K5 K4 O21 51.6(7) . 3_575
O48 K4 O21 156.0(15) . 3_575
O35 K4 O21 94.3(9) 3_676 3_575
O18 K4 O21 52.9(5) 3_575 3_575
O40 K4 O21 124.3(13) . 3_575
O23 K4 O21 65.0(7) 3_676 3_575
O2B K4 O21 115.8(12) 3_575 3_575
K5 K4 C2A 155.9(12) . 2
O48 K4 C2A 55.8(15) . 2
O35 K4 C2A 75.5(10) 3_676 2
O18 K4 C2A 60.8(8) 3_575 2
O40 K4 C2A 118.9(13) . 2
O23 K4 C2A 129.9(11) 3_676 2
O2B K4 C2A 14.4(10) 3_575 2
O21 K4 C2A 112.3(8) 3_575 2
K5 K4 O8 92.0(10) . 3_676
O48 K4 O8 62.1(13) . 3_676
O35 K4 O8 53.1(6) 3_676 3_676
O18 K4 O8 121.8(10) 3_575 3_676
O40 K4 O8 66.9(9) . 3_676
O23 K4 O8 48.0(5) 3_676 3_676
O2B K4 O8 98.3(12) 3_575 3_676
O21 K4 O8 112.9(9) 3_575 3_676
C2A K4 O8 111.8(11) 2 3_676
K5 K4 W8 95.9(10) . 3_676
O48 K4 W8 73.6(13) . 3_676
O35 K4 W8 28.4(5) 3_676 3_676
O18 K4 W8 90.8(7) 3_575 3_676
O40 K4 W8 97.6(9) . 3_676
O23 K4 W8 32.9(4) 3_676 3_676
O2B K4 W8 88.6(12) 3_575 3_676
O21 K4 W8 91.2(7) 3_575 3_676
C2A K4 W8 102.8(10) 2 3_676
O8 K4 W8 31.4(3) 3_676 3_676
K5 K4 W9 78.1(7) . 3_575
O48 K4 W9 132.2(14) . 3_575
O35 K4 W9 80.2(7) 3_676 3_575
O18 K4 W9 26.5(3) 3_575 3_575
O40 K4 W9 150.5(13) . 3_575
O23 K4 W9 74.9(6) 3_676 3_575
O2B K4 W9 89.3(11) 3_575 3_575
O21 K4 W9 26.5(3) 3_575 3_575
C2A K4 W9 86.9(7) 2 3_575
O8 K4 W9 119.1(8) 3_676 3_575
W8 K4 W9 89.3(5) 3_676 3_575
K5 K6 O17 85.4(9) . .
K5 K6 O43 89.1(16) . .
O17 K6 O43 82.1(11) . .
K5 K6 O41 112.0(13) . .
O17 K6 O41 101.9(12) . .
O43 K6 O41 158.6(16) . .
K5 K6 O11 154.1(16) . 1_554
O17 K6 O11 103.0(13) . 1_554
O43 K6 O11 68.3(11) . 1_554
O41 K6 O11 90.4(11) . 1_554
K5 K6 O43 94.2(18) . 3_675
O17 K6 O43 169.3(12) . 3_675
O43 K6 O43 87.2(14) . 3_675
O41 K6 O43 88.2(10) . 3_675
O11 K6 O43 73.1(11) 1_554 3_675
K5 K6 O21 52.4(10) . 3_575
O17 K6 O21 129.3(10) . 3_575
O43 K6 O21 118.7(17) . 3_575
O41 K6 O21 75.2(7) . 3_575
O11 K6 O21 127.5(9) 1_554 3_575
O43 K6 O21 56.5(11) 3_675 3_575
K5 K6 K2 70.0(9) . .
O17 K6 K2 43.2(4) . .
O43 K6 K2 44.1(9) . .
O41 K6 K2 144.9(11) . .
O11 K6 K2 99.3(7) 1_554 .
O43 K6 K2 126.9(13) 3_675 .
O21 K6 K2 121.4(11) 3_575 .
K5 K6 K3 120.8(12) . 1_554
O17 K6 K3 136.5(13) . 1_554
O43 K6 K3 127.8(11) . 1_554
O41 K6 K3 38.5(5) . 1_554
O11 K6 K3 69.2(6) 1_554 1_554
O43 K6 K3 52.1(9) 3_675 1_554
O21 K6 K3 68.7(5) 3_575 1_554
K2 K6 K3 168.5(9) . 1_554
K5 K6 K6 92.3(18) . 3_675
O17 K6 K6 126.9(9) . 3_675
O43 K6 K6 44.8(10) . 3_675
O41 K6 K6 127.4(9) . 3_675
O11 K6 K6 62.9(7) 1_554 3_675
O43 K6 K6 42.4(10) 3_675 3_675
O21 K6 K6 86.2(13) 3_575 3_675
K2 K6 K6 86.5(7) . 3_675
K3 K6 K6 88.9(6) 1_554 3_675
K5 K6 K4 23.4(10) . .
O17 K6 K4 86.2(7) . .
O43 K6 K4 112.4(14) . .
O41 K6 K4 88.9(7) . .
O11 K6 K4 170.7(12) 1_554 .
O43 K6 K4 97.6(14) 3_675 .
O21 K6 K4 43.6(5) 3_575 .
K2 K6 K4 86.5(6) . .
K3 K6 K4 105.0(6) 1_554 .
K6 K6 K4 110.5(16) 3_675 .
K5 K6 K5 120.2(15) . 3_675
O17 K6 K5 123.9(9) . 3_675
O43 K6 K5 52.7(10) . 3_675
O41 K6 K5 110.5(8) . 3_675
O11 K6 K5 35.5(6) 1_554 3_675
O43 K6 K5 47.7(10) 3_675 3_675
O21 K6 K5 103.2(8) 3_575 3_675
K2 K6 K5 96.1(5) . 3_675
K3 K6 K5 75.2(5) 1_554 3_675
K6 K6 K5 27.8(7) 3_675 3_675
K4 K6 K5 137.1(11) . 3_675
K3 O37 K3 179.998(2) . 3_576
K3 O37 K1 92.5(3) . .
K3 O37 K1 87.5(3) 3_576 .
K3 O37 K1 87.5(3) . 3_576
K3 O37 K1 92.5(3) 3_576 3_576
K1 O37 K1 180.000(1) . 3_576
O38 O38 K1 167.2(7) 4_585 .
O40 O39 K5 103(2) . .
O40 O39 K2 173(2) . .
K5 O39 K2 83.1(12) . .
O39 O40 K4 106(2) . .
O39 O40 K1 169(2) . .
K4 O40 K1 84.7(11) . .
O39 O40 K5 54.8(18) . .
K4 O40 K5 51.4(10) . .
K1 O40 K5 135.8(13) . .
K2 O43 K6 88.8(14) . .
K2 O43 K6 155.8(19) . 3_675
K6 O43 K6 92.8(14) . 3_675
K2 O43 K3 82.5(11) . 3_676
K6 O43 K3 144.4(18) . 3_676
K6 O43 K3 82.2(13) 3_675 3_676
K2 O44 K2 176.2(12) . 4_575
K6 K5 O21 83.5(11) . 3_575
K6 K5 K4 136.8(15) . .
O21 K5 K4 74.2(11) 3_575 .
K6 K5 O39 116.2(15) . .
O21 K5 O39 153(2) 3_575 .
K4 K5 O39 78.5(12) . .
K6 K5 O11 94.0(15) . 3_676
O21 K5 O11 77.1(8) 3_575 3_676
K4 K5 O11 115.6(13) . 3_676
O39 K5 O11 117.6(11) . 3_676
K6 K5 O23 142.2(14) . 3_676
O21 K5 O23 72.2(9) 3_575 3_676
K4 K5 O23 63.5(10) . 3_676
O39 K5 O23 97.4(12) . 3_676
O11 K5 O23 53.1(6) 3_676 3_676
K6 K5 O40 130.6(14) . .
O21 K5 O40 129.9(18) 3_575 .
K4 K5 O40 55.8(10) . .
O39 K5 O40 22.7(9) . .
O11 K5 O40 124.9(11) 3_676 .
O23 K5 O40 86.9(12) 3_676 .
K6 K5 O9 129.0(17) . 3_676
O21 K5 O9 115.1(10) 3_575 3_676
K4 K5 O9 94.1(11) . 3_676
O39 K5 O9 68.5(8) . 3_676
O11 K5 O9 50.9(6) 3_676 3_676
O23 K5 O9 47.3(5) 3_676 3_676
O40 K5 O9 74.5(9) . 3_676
K6 K5 W7 121.1(16) . 3_676
O21 K5 W7 85.5(8) 3_575 3_676
K4 K5 W7 93.8(11) . 3_676
O39 K5 W7 98.4(9) . 3_676
O11 K5 W7 27.4(4) 3_676 3_676
O23 K5 W7 31.0(4) 3_676 3_676
O40 K5 W7 99.5(10) . 3_676
O9 K5 W7 30.7(3) 3_676 3_676
K6 K5 K2 75.5(11) . .
O21 K5 K2 156.3(16) 3_575 .
K4 K5 K2 129.1(10) . .
O39 K5 K2 50.7(7) . .
O11 K5 K2 93.3(10) 3_676 .
O23 K5 K2 119.2(8) 3_676 .
O40 K5 K2 73.4(8) . .
O9 K5 K2 71.9(6) 3_676 .
W7 K5 K2 95.8(7) 3_676 .
K6 K5 K6 59.8(15) . 3_675
O21 K5 K6 81.1(9) 3_575 3_675
K4 K5 K6 146.4(11) . 3_675
O39 K5 K6 124.6(12) . 3_675
O11 K5 K6 34.8(8) 3_676 3_675
O23 K5 K6 87.5(9) 3_676 3_675
O40 K5 K6 144.4(11) . 3_675
O9 K5 K6 76.0(8) 3_676 3_675
W7 K5 K6 61.3(7) 3_676 3_675
K2 K5 K6 78.9(8) . 3_675
K3 O41 K6 96.3(8) 1_554 .
K3 O45 K2 119(4) . 3_676
K1 O48 K4 108(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O13 1.713(11) .
W1 O14 1.850(12) .
W1 O16 1.887(11) .
W1 O30 1.909(7) .
W1 O1 1.952(11) .
W1 O36 2.361(10) .
W1 K3 3.678(15) 3_576
W1 K1 3.995(6) 3_576
W2 O17 1.737(12) .
W2 O19 1.787(13) .
W2 O31 1.916(5) .
W2 O15 1.932(12) .
W2 O3 2.022(12) .
W2 O22 2.383(10) .
W2 K2 3.882(5) .
W3 O12 1.709(11) .
W3 O1 1.874(12) .
W3 O5 1.886(12) .
W3 O29 1.909(7) .
W3 O10 1.936(13) .
W3 O26 2.353(10) .
W3 K3 3.583(14) .
W3 K1 3.881(6) 3_576
W4 O20 1.714(13) .
W4 O24 1.889(14) .
W4 O15 1.905(12) .
W4 O16 1.919(11) .
W4 O2 1.921(13) .
W4 O22 2.341(10) .
W4 K3 3.810(15) 3_576
W4 K1 3.999(6) .
W5 O6 1.734(11) .
W5 O3 1.845(12) .
W5 O27 1.883(3) .
W5 O4 1.921(13) .
W5 O8 1.978(12) .
W5 O7 2.375(10) .
W5 K2 3.821(6) .
W6 O25 1.704(14) .
W6 O5 1.903(12) .
W6 O2 1.906(13) .
W6 O4 1.930(14) .
W6 O9 1.944(15) .
W6 O7 2.355(11) .
W6 K1 3.847(7) .
W6 K3 3.958(16) .
W9 O21 1.725(14) .
W9 O18 1.807(13) .
W9 O34 1.914(8) .
W9 O24 1.952(14) .
W9 O14 1.999(12) .
W9 O32 2.395(9) .
W9 K4 3.848(19) 3_575
W8 O35 1.72(2) .
W8 O8 1.885(14) .
W8 O8 1.885(14) 4_575
W8 O23 1.946(15) 4_575
W8 O23 1.946(15) .
W8 O28 2.375(16) .
W8 K4 3.57(3) 3_676
W8 K4 3.57(3) 2_646
W7 O11 1.700(14) .
W7 O23 1.891(14) .
W7 O9 1.895(15) .
W7 O10 1.903(12) .
W7 O33 1.917(9) .
W7 O28 2.371(11) .
W7 K5 3.68(3) 3_676
Ru1 O19 2.011(14) 4_575
Ru1 O19 2.011(14) .
Ru1 O18 2.020(14) 4_575
Ru1 O18 2.020(14) .
Ru1 S1 2.044(9) .
Ru1 O32 2.256(14) .
P1 O26 1.521(15) .
P1 O7 1.525(11) .
P1 O7 1.525(11) 4_575
P1 O28 1.590(17) .
P2 O36 1.528(15) .
P2 O22 1.534(10) .
P2 O22 1.534(10) 4_575
P2 O32 1.591(13) .
S1 O2B 1.61(5) .
S1 O2B 1.61(5) 4_575
S1 C2A 1.79(3) 4_575
S1 C2A 1.79(3) .
S1 C70A 1.81(3) .
S1 C70A 1.81(3) 4_575
C70A H70A 0.9800 .
C70A H70B 0.9800 .
C70A H70C 0.9800 .
C2A K4 3.32(5) 2_545
C2A H2A1 0.9800 .
C2A H2A2 0.9800 .
C2A H2A3 0.9800 .
O2B K4 3.24(6) 3_575
O1 K1 3.360(12) 3_576
O2 K1 3.369(13) .
O3 K2 3.281(11) .
O5 K3 3.13(2) .
O6 K2 2.755(14) .
O6 K1 2.795(13) 3_676
O8 K4 3.36(3) 3_676
O9 K5 3.43(3) 3_676
O11 K6 3.04(4) 1_556
O11 K5 3.09(3) 3_676
O12 K3 2.642(19) .
O12 K1 2.780(15) 3_576
O13 K2 2.747(13) 1_455
O13 K3 2.848(19) 3_576
O13 K1 2.902(15) 3_576
O16 K3 3.114(19) 3_576
O17 K2 2.736(15) .
O17 K6 2.88(3) .
O18 K4 2.89(2) 3_575
O20 K1 2.904(17) .
O20 K3 3.06(2) 3_576
O21 K5 2.66(3) 3_575
O21 K4 3.27(3) 3_575
O21 K6 3.34(4) 3_575
O23 K4 3.12(3) 3_676
O23 K5 3.14(4) 3_676
O25 K1 2.700(18) .
O25 K2 2.767(15) 3_676
O25 K3 3.29(2) .
O26 W3 2.353(10) 4_575
O27 W5 1.883(3) 4_575
O28 W7 2.371(11) 4_575
O29 W3 1.909(7) 4_575
O30 W1 1.909(7) 4_575
O31 W2 1.916(5) 4_575
O32 W9 2.395(9) 4_575
O33 W7 1.917(9) 4_575
O34 W9 1.914(8) 4_575
O35 K4 2.88(3) 3_676
O35 K4 2.88(3) 2_646
O36 W1 2.361(10) 4_575
K1 O48 2.31(6) .
K1 O12 2.780(15) 3_576
K1 O6 2.795(13) 3_676
K1 O13 2.902(15) 3_576
K1 O38 3.02(4) .
K1 O40 3.28(4) .
K1 O37 3.293(7) .
K1 O1 3.360(12) 3_576
K2 O13 2.747(13) 1_655
K2 O25 2.767(15) 3_676
K2 O43 2.78(5) .
K2 O46 2.81(7) .
K2 O39 3.03(3) .
K2 O44 3.149(6) .
K2 O45 3.42(6) 3_676
K2 K5 3.88(3) .
K3 O45 1.12(6) .
K3 O41 2.65(3) 1_556
K3 O13 2.848(19) 3_576
K3 O37 2.91(2) .
K3 O20 3.06(2) 3_576
K3 O16 3.114(19) 3_576
K3 O43 3.37(5) 3_676
K3 W1 3.678(15) 3_576
K4 K5 2.76(5) .
K4 O48 2.84(6) .
K4 O35 2.88(3) 3_676
K4 O18 2.89(2) 3_575
K4 O40 2.92(4) .
K4 O23 3.12(3) 3_676
K4 O2B 3.24(6) 3_575
K4 O21 3.27(3) 3_575
K4 C2A 3.32(5) 2
K4 O8 3.36(3) 3_676
K4 W8 3.57(3) 3_676
K4 W9 3.848(19) 3_575
K6 K5 2.34(6) .
K6 O43 2.93(5) .
K6 O41 3.02(3) .
K6 O11 3.04(4) 1_554
K6 O43 3.06(5) 3_675
K6 O21 3.34(4) 3_575
K6 K3 4.23(3) 1_554
K6 K6 4.33(6) 3_675
K6 K5 5.01(5) 3_675
O37 K3 2.91(2) 3_576
O37 K1 3.293(7) 3_576
O38 O38 0.94(7) 4_585
O39 O40 1.33(4) .
O39 K5 2.82(4) .
O40 K5 3.37(5) .
O43 K6 3.06(5) 3_675
O43 K3 3.37(5) 3_676
O44 K2 3.149(6) 4_575
K5 O21 2.66(3) 3_575
K5 O11 3.09(3) 3_676
K5 O23 3.14(4) 3_676
K5 O9 3.43(3) 3_676
K5 W7 3.68(3) 3_676
K5 K6 5.01(5) 3_675
O41 K3 2.65(3) 1_554
O45 K2 3.42(6) 3_676
